Luminescence, Chemical Sensing and Mechanical Properties of Crystalline Materials Based on Lanthanide-Sulfonate Coordination Polymers
D'Vries, Richard Fernando; Gómez, Germán; Lionello, Diego E.; Fuertes, Cecilia; Soler-Illia, Galo; Ellena, Javier A.; RSC Adv.  (2016) –; doi:10.1039/C6RA23516F

data_7227083
_publ_section_title
;
 Luminescence, Chemical Sensing and Mechanical Properties of Crystalline
 Materials Based on Lanthanide-Sulfonate Coordination Polymers
;
_journal_name_full               'RSC Adv.'
_journal_paper_doi               10.1039/C6RA23516F
_journal_year                    2016
_chemical_formula_moiety         'C44 H28 N4 O15 S4 Tb2, 3(H2 O)'
_chemical_formula_sum            'C44 H34 N4 O18 S4 Tb2'
_chemical_formula_weight         1352.83
_space_group_crystal_system      monoclinic
_space_group_IT_number           14
_space_group_name_Hall           '-P 2yn'
_space_group_name_H-M_alt        'P 1 21/n 1'
_symmetry_space_group_name_Hall  '-P 2yn'
_symmetry_space_group_name_H-M   'P 1 21/n 1'
_atom_sites_solution_hydrogens   mixed
_audit_creation_date             2015-10-14
_audit_creation_method
;
Olex2 1.2
(compiled 2015.09.30 svn.r3233 for OlexSys, GUI svn.r5103)
;
_audit_update_record
;
2016-05-03 deposited with the CCDC.
2016-11-10 downloaded from the CCDC.
;
_cell_angle_alpha                90
_cell_angle_beta                 99.088(2)
_cell_angle_gamma                90
_cell_formula_units_Z            4
_cell_length_a                   14.2636(6)
_cell_length_b                   17.0354(7)
_cell_length_c                   18.9491(7)
_cell_measurement_reflns_used    9937
_cell_measurement_temperature    296(2)
_cell_measurement_theta_max      24.12
_cell_measurement_theta_min      2.28
_cell_volume                     4546.6(3)
_computing_cell_refinement       'SAINT v8.34A (Bruker, 2013)'
_computing_data_collection       'Bruker APEX2'
_computing_data_reduction        'SAINT v8.34A (Bruker, 2013)'
_computing_molecular_graphics    'Olex2 (Dolomanov et al., 2009)'
_computing_publication_material  'Olex2 (Dolomanov et al., 2009)'
_computing_structure_refinement  'ShelXL (Sheldrick, 2015)'
_computing_structure_solution    'ShelXS (Sheldrick, 20015)'
_diffrn_ambient_temperature      296
_diffrn_measured_fraction_theta_full 1.000
_diffrn_measured_fraction_theta_max 0.994
_diffrn_measurement_device_type  'Bruker APEX-II CCD'
_diffrn_measurement_method       '\f and \w scans'
_diffrn_radiation_type           MoK\a
_diffrn_radiation_wavelength     0.71073
_diffrn_reflns_av_R_equivalents  0.1040
_diffrn_reflns_av_unetI/netI     0.0435
_diffrn_reflns_Laue_measured_fraction_full 1.000
_diffrn_reflns_Laue_measured_fraction_max 0.994
_diffrn_reflns_limit_h_max       17
_diffrn_reflns_limit_h_min       -17
_diffrn_reflns_limit_k_max       21
_diffrn_reflns_limit_k_min       -21
_diffrn_reflns_limit_l_max       23
_diffrn_reflns_limit_l_min       -23
_diffrn_reflns_number            140387
_diffrn_reflns_point_group_measured_fraction_full 1.000
_diffrn_reflns_point_group_measured_fraction_max 0.994
_diffrn_reflns_theta_full        26.000
_diffrn_reflns_theta_max         26.493
_diffrn_reflns_theta_min         1.617
_diffrn_standards_number         0
_exptl_absorpt_coefficient_mu    3.354
_exptl_absorpt_correction_T_max  0.7454
_exptl_absorpt_correction_T_min  0.6118
_exptl_absorpt_correction_type   multi-scan
_exptl_absorpt_process_details
;
SADABS-2014/5 (Bruker,2014/5) was used for absorption correction.
wR2(int) was 0.1206 before and 0.0694 after correction.
The Ratio of minimum to maximum transmission is 0.8208.
The \l/2 correction factor is 0.00150.
;
_exptl_crystal_colour            'clear light yellow'
_exptl_crystal_colour_lustre     clear
_exptl_crystal_colour_modifier   light
_exptl_crystal_colour_primary    yellow
_exptl_crystal_density_diffrn    1.976
_exptl_crystal_description       needle
_exptl_crystal_F_000             2656
_exptl_crystal_preparation       Luminescent
_exptl_crystal_recrystallization_method Hydrothermal
_exptl_crystal_size_max          0.22
_exptl_crystal_size_mid          0.05
_exptl_crystal_size_min          0.04
_refine_diff_density_max         1.687
_refine_diff_density_min         -1.531
_refine_diff_density_rms         0.149
_refine_ls_extinction_method     none
_refine_ls_goodness_of_fit_ref   1.119
_refine_ls_hydrogen_treatment    constr
_refine_ls_matrix_type           full
_refine_ls_number_parameters     647
_refine_ls_number_reflns         9363
_refine_ls_number_restraints     0
_refine_ls_restrained_S_all      1.119
_refine_ls_R_factor_all          0.0678
_refine_ls_R_factor_gt           0.0365
_refine_ls_shift/su_max          0.001
_refine_ls_shift/su_mean         0.000
_refine_ls_structure_factor_coef Fsqd
_refine_ls_weighting_details
'w=1/[\s^2^(Fo^2^)+(0.0325P)^2^+14.2315P] where P=(Fo^2^+2Fc^2^)/3'
_refine_ls_weighting_scheme      calc
_refine_ls_wR_factor_gt          0.0765
_refine_ls_wR_factor_ref         0.0927
_reflns_Friedel_coverage         0.000
_reflns_number_gt                6857
_reflns_number_total             9363
_reflns_threshold_expression     'I > 2\s(I)'
_cod_data_source_file            c6ra23516f2.cif
_cod_data_source_block           Phase3-Tb
_cod_database_code               7227083
_olex2_refinement_description
;
1. Fixed Uiso
 At 1.2 times of:
  All C(H) groups
 At 1.5 times of:
  All O(H,H) groups
2.a Free rotating group:
 O16(H16A,H16B,O17,H17A,H17B,O18,H18A,H18B)
2.b Rotating group:
 O15(H15A,H15B)
2.c Aromatic/amide H refined with riding coordinates:
 C2(H2), C4(H4), C6(H6), C7(H7), C9(H9), C12(H12), C14(H14), C15(H15),
 C17(H17), C19(H19), C21(H21), C22(H22), C23(H23), C25(H25), C26(H26), C28(H28),
  C29(H29), C30(H30), C33(H33), C34(H34), C35(H35), C37(H37), C38(H38),
 C40(H40), C41(H41), C42(H42)
;
_shelx_res_checksum              92076
_shelx_shelxl_version_number     2014/7
_olex2_submission_special_instructions 'No special instructions were received'